Table 15. Continued. 



Alloy 



CDA 



No." 



Environment 



Exposure 



(day) 



Depth 



(ft) 



Corrosion 

 Rate 

 (mpy) 



Type of 

 Corrosion c 



Source 



Yellow Brass 



270 



W 



1,064 



5,300 



0.6 



U 



INCO (3) 



Yellow Brass 



270 



S 



1,064 



5,300 



0.5 



U 



INCO(3) 



Yellow Brass 



270 



W 



197 



2,340 



0.9 



U 



INCO (3) 



Yellow Brass 



270 



s 



197 



2,340 



0.2 



NU-ET 



INCO (3) 



Yellow Brass 



270 



w 



402 



2,370 



0.9 



U 



INCO (3) 



Yellow Brass 



270 



s 



402 



2,370 



0.1 



ET 



INCO (3) 



Yellow Brass 



270 



w 



181 



5 



2.1 



U 



INCO (3) 



Yellow Brass 



270 



w 



366 



5 



1.3 



U 



INCO (3) 



Muntz Metal 



280 



w 



123 



5,640 



1.6 



SL-DZ 



CEL (4) 



Muntz Metal 



280 



w 



123 



5,640 



2.1 



U 



INCO (3) 



Muntz Metal 



280 



s 



123 



5,640 



1.3 



SL-DZ 



CEL (4) 



Muntz Metal 



280 



s 



123 



5,640 



1.5 



U 



INCO (3) 



Muntz Metal 



280 



w 



403 



6,780 



2.6 



SL-DZ 



CEL (4) 



Muntz Metal 



280 



w 



403 



6,780 



3.3 



S-DZ 



INCO (3) 



Muntz Metal 



280 



s 



403 



6,780 



1.8 



SL-DZ 



CEL (4) 



Muntz Metal 



280 



s 



403 



6,780 



0.6 



GBSL 



INCO (3) 



Muntz Metal 



280 



w 



751 



5,640 



3.2 



G-DZ 



CEL (4) 



Muntz Metal 



280 



w 



751 



5,640 



4.0 



S-DZ 



INCO (3) 



Muntz Metal 



280 



s 



751 



5,640 



1.7 



S-DZ 



INCO (3) 



Muntz Metal 



280 



w 



1,064 



5,300 



2.3 



S-DZ 



INCO (3) 



Muntz Metal 



280 



s 



1,064 



5,300 



0.8 



U 



INCO (3) 



Muntz Metal 



280 



w 



197 



2,340 



0.7 



SL-DZ; P (10) 



CEL (4) 



Muntz Metal 



280 



w 



197 



2,340 



0.7 



U 



INCO (3) 



Muntz Metal 



280 



s 



197 



2,340 



0.5 



SL-DZ; P (5) 



CEL (4) 



Muntz Metal 



280 



s 



197 



2,340 



<0.1 



SL-DZ^ 



INCO (3) 



Muntz Metal 



280 



w 



402 



2,370 



0.7 



SL-DZ 



CEL (4) 



Muntz Metal 



280 



w 



402 



2,370 



0.7 



SL-DZ 



INCO (3) 



Muntz Metal 



280 



s 



402 



2,370 



0.6 



SL-DZ 



CEL (4) 



Muntz Metal 



280 



s 



402 



2,370 



0.1 



ET 



INCO (3) 



Muntz Metal 



280 



w 



181 



5 



2.4 



DZ 



CEL (4) 



Muntz Metal 



280 



w 



181 



5 



3.4 



SL-DZ 



INCO (3) 



Muntz Metal 



280 



w 



366 



5 



3.7 



S-DZ 



INCO (3) 



Muntz Metal 



280 



w 



398 



5 



3.1 



DZ, P(6) 



CEL (4) 



Muntz Metal 



280 



w 



540 



5 



3.4 



DZ, IP 



CEL (4) 



Muntz Metal 



280 



w 



588 



5 



3.3 



DZ, I-P 



CEL (4) 



Arsenical Admiralty 



443 



w 



123 



5,640 



1.0 



U 



CEL (4) 



Arsenical Admiralty 



443 



w 



123 



5,640 



1.1 



u 



INCO (3) 



Arsenical Admiralty 



443 



s 



123 



5,640 



1.0 



u 



CEL (4) 



Arsenical Admiralty 



443 



s 



123 



5,640 



1.0 



u 



INCO (3) 



Arsenical Admiralty 



443 



w 



403 



6,780 



0.7 



u 



CEL (4) 



Arsenical Admiralty 



443 



w 



403 



6,780 



0.8 



u 



INCO (3) 



Continued 



64 



